#------------------------------------------------------------------------------
#$Date: 2016-03-23 16:56:26 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179400 $
#$URL: svn://www.crystallography.net/cod/cif/4/32/97/4329780.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4329780
loop_
_publ_author_name
'Chun-Liang Chen'
'Quang Bac Nguyen'
'Chih-Shan Chen'
'Kwang-Hwa Lii'
_publ_section_title
;
 Mixed-Valence Uranium Germanate and Silicate: Csx(UVO)(UIV/VO)2(Ge2O7)2
 (x = 3.18) and Cs4(UVO)(UIV/VO)2(Si2O7)2
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              7463
_journal_page_last               7465
_journal_paper_doi               10.1021/ic301091f
_journal_volume                  51
_journal_year                    2012
_chemical_formula_moiety         Cs4(UO)(UO)2(Si2O7)2
_chemical_formula_sum            'Cs4 O17 Si4 U3'
_chemical_formula_weight         1630.09
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 107.43(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   11.594(2)
_cell_length_b                   7.5438(15)
_cell_length_c                   11.894(2)
_cell_measurement_temperature    293(2)
_cell_volume                     992.5(4)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    Diamond
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0369
_diffrn_reflns_av_sigmaI/netI    0.0261
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            3711
_diffrn_reflns_theta_full        28.21
_diffrn_reflns_theta_max         28.21
_diffrn_reflns_theta_min         1.79
_exptl_absorpt_coefficient_mu    31.962
_exptl_absorpt_correction_T_max  0.985
_exptl_absorpt_correction_T_min  0.345
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    5.455
_exptl_crystal_description       plate
_exptl_crystal_F_000             1376
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.04
_refine_diff_density_max         1.526
_refine_diff_density_min         -3.233
_refine_diff_density_rms         0.348
_refine_ls_extinction_coef       0.00111(9)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.133
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     76
_refine_ls_number_reflns         1315
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.133
_refine_ls_R_factor_all          0.0253
_refine_ls_R_factor_gt           0.0247
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0391P)²+8.1704P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0656
_refine_ls_wR_factor_ref         0.0661
_reflns_number_gt                1284
_reflns_number_total             1315
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic301091f_si_003_2.cif
_cod_data_source_block           csusio
_cod_original_cell_volume        992.5(3)
_cod_database_code               4329780
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Cs1 Cs 0.82101(6) 0.0000 0.48252(5) 0.02568(17) Uani 1 2 d S
Cs2 Cs 0.85172(5) 0.0000 0.07976(6) 0.02352(16) Uani 1 2 d S
U1 U 0.5000 0.0000 0.0000 0.00804(13) Uani 1 4 d S
U2 U 0.44973(2) 0.0000 0.31245(2) 0.00776(12) Uani 1 2 d S
Si1 Si 0.66066(12) -0.2940(2) 0.23293(13) 0.0091(3) Uani 1 1 d .
O1 O 0.6230(4) -0.2018(6) 0.1040(4) 0.0175(9) Uani 1 1 d .
O2 O 0.8056(3) -0.2946(6) 0.2969(4) 0.0159(8) Uani 1 1 d .
O3 O 0.5907(4) -0.2013(6) 0.3181(4) 0.0174(9) Uani 1 1 d .
O4 O 0.6145(6) -0.5000 0.2140(7) 0.0228(15) Uani 1 2 d S
O5 O 0.4049(5) 0.0000 0.1210(6) 0.0164(12) Uani 1 2 d S
O6 O 0.5000 0.0000 0.5000 0.033(3) Uani 1 4 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 Cs1 O2 91.60(17) . 6
O2 Cs1 O3 50.33(11) . .
O2 Cs1 O3 92.62(11) 6 .
O2 Cs1 O3 92.62(11) . 6
O2 Cs1 O3 50.33(10) 6 6
O3 Cs1 O3 57.00(16) . 6
O2 Cs1 O3 165.34(11) . 4_656
O2 Cs1 O3 87.74(12) 6 4_656
O3 Cs1 O3 144.33(7) . 4_656
O3 Cs1 O3 98.18(10) 6 4_656
O2 Cs1 O3 87.74(11) . 7_646
O2 Cs1 O3 165.34(11) 6 7_646
O3 Cs1 O3 98.18(10) . 7_646
O3 Cs1 O3 144.33(7) 6 7_646
O3 Cs1 O3 89.21(16) 4_656 7_646
O2 Cs1 O4 133.74(8) . 7_646
O2 Cs1 O4 133.74(8) 6 7_646
O3 Cs1 O4 121.35(12) . 7_646
O3 Cs1 O4 121.35(12) 6 7_646
O3 Cs1 O4 46.17(8) 4_656 7_646
O3 Cs1 O4 46.17(8) 7_646 7_646
O2 Cs1 Si1 159.22(9) . 4_656
O2 Cs1 Si1 109.15(9) 6 4_656
O3 Cs1 Si1 125.07(8) . 4_656
O3 Cs1 Si1 99.83(9) 6 4_656
O3 Cs1 Si1 26.36(8) 4_656 4_656
O3 Cs1 Si1 72.44(9) 7_646 4_656
O4 Cs1 Si1 26.32(4) 7_646 4_656
O2 Cs1 Si1 109.15(9) . 7_646
O2 Cs1 Si1 159.22(9) 6 7_646
O3 Cs1 Si1 99.83(9) . 7_646
O3 Cs1 Si1 125.07(8) 6 7_646
O3 Cs1 Si1 72.44(9) 4_656 7_646
O3 Cs1 Si1 26.36(8) 7_646 7_646
O4 Cs1 Si1 26.32(4) 7_646 7_646
Si1 Cs1 Si1 50.08(5) 4_656 7_646
O2 Cs1 O2 148.55(9) . 4_656
O2 Cs1 O2 104.70(9) 6 4_656
O3 Cs1 O2 101.37(10) . 4_656
O3 Cs1 O2 78.36(10) 6 4_656
O3 Cs1 O2 44.75(10) 4_656 4_656
O3 Cs1 O2 82.92(10) 7_646 4_656
O4 Cs1 O2 43.06(11) 7_646 4_656
Si1 Cs1 O2 25.42(7) 4_656 4_656
Si1 Cs1 O2 56.67(7) 7_646 4_656
O2 Cs1 O2 104.70(9) . 7_646
O2 Cs1 O2 148.55(9) 6 7_646
O3 Cs1 O2 78.36(10) . 7_646
O3 Cs1 O2 101.37(10) 6 7_646
O3 Cs1 O2 82.92(10) 4_656 7_646
O3 Cs1 O2 44.75(10) 7_646 7_646
O4 Cs1 O2 43.06(11) 7_646 7_646
Si1 Cs1 O2 56.67(7) 4_656 7_646
Si1 Cs1 O2 25.42(7) 7_646 7_646
O2 Cs1 O2 49.41(13) 4_656 7_646
O2 Cs1 Si1 25.47(7) . .
O2 Cs1 Si1 87.17(8) 6 .
O3 Cs1 Si1 25.83(8) . .
O3 Cs1 Si1 70.61(9) 6 .
O3 Cs1 Si1 168.39(8) 4_656 .
O3 Cs1 Si1 98.25(9) 7_646 .
O4 Cs1 Si1 137.02(6) 7_646 .
Si1 Cs1 Si1 149.73(3) 4_656 .
Si1 Cs1 Si1 111.09(3) 7_646 .
O2 Cs1 Si1 127.14(7) 4_656 .
O2 Cs1 Si1 96.10(7) 7_646 .
O4 Cs2 O1 134.78(14) 3 .
O4 Cs2 O1 134.78(14) 3 6
O1 Cs2 O1 57.89(16) . 6
O4 Cs2 O5 165.44(19) 3 5_655
O1 Cs2 O5 56.56(12) . 5_655
O1 Cs2 O5 56.56(12) 6 5_655
O4 Cs2 O1 94.43(14) 3 7_645
O1 Cs2 O1 88.56(11) . 7_645
O1 Cs2 O1 130.77(7) 6 7_645
O5 Cs2 O1 75.34(11) 5_655 7_645
O4 Cs2 O1 94.43(14) 3 4_655
O1 Cs2 O1 130.77(7) . 4_655
O1 Cs2 O1 88.56(11) 6 4_655
O5 Cs2 O1 75.34(11) 5_655 4_655
O1 Cs2 O1 88.97(15) 7_645 4_655
O4 Cs2 O2 87.89(14) 3 6
O1 Cs2 O2 85.51(10) . 6
O1 Cs2 O2 47.05(10) 6 6
O5 Cs2 O2 103.42(11) 5_655 6
O1 Cs2 O2 173.50(10) 7_645 6
O1 Cs2 O2 96.92(10) 4_655 6
O4 Cs2 O2 87.89(14) 3 .
O1 Cs2 O2 47.05(10) . .
O1 Cs2 O2 85.51(10) 6 .
O5 Cs2 O2 103.42(11) 5_655 .
O1 Cs2 O2 96.92(10) 7_645 .
O1 Cs2 O2 173.50(10) 4_655 .
O2 Cs2 O2 77.08(13) 6 .
O4 Cs2 O4 97.33(18) 3 7_645
O1 Cs2 O4 115.17(12) . 7_645
O1 Cs2 O4 115.17(12) 6 7_645
O5 Cs2 O4 68.11(15) 5_655 7_645
O1 Cs2 O4 44.49(8) 7_645 7_645
O1 Cs2 O4 44.49(8) 4_655 7_645
O2 Cs2 O4 141.23(7) 6 7_645
O2 Cs2 O4 141.23(7) . 7_645
O4 Cs2 O1 43.29(10) 3 3
O1 Cs2 O1 168.31(15) . 3
O1 Cs2 O1 114.03(3) 6 3
O5 Cs2 O1 128.11(10) 5_655 3
O1 Cs2 O1 102.93(10) 7_645 3
O1 Cs2 O1 52.81(13) 4_655 3
O2 Cs2 O1 82.91(9) 6 3
O2 Cs2 O1 127.81(9) . 3
O4 Cs2 O1 75.41(10) 7_645 3
O4 Cs2 O1 43.29(10) 3 8_545
O1 Cs2 O1 114.03(3) . 8_545
O1 Cs2 O1 168.31(15) 6 8_545
O5 Cs2 O1 128.11(10) 5_655 8_545
O1 Cs2 O1 52.81(13) 7_645 8_545
O1 Cs2 O1 102.93(10) 4_655 8_545
O2 Cs2 O1 127.81(9) 6 8_545
O2 Cs2 O1 82.91(9) . 8_545
O4 Cs2 O1 75.41(10) 7_645 8_545
O1 Cs2 O1 72.46(13) 3 8_545
O4 Cs2 Si1 23.97(2) 3 3
O1 Cs2 Si1 147.92(8) . 3
O1 Cs2 Si1 117.02(8) 6 3
O5 Cs2 Si1 151.75(6) 5_655 3
O1 Cs2 Si1 110.19(8) 7_645 3
O1 Cs2 Si1 77.07(8) 4_655 3
O2 Cs2 Si1 73.99(7) 6 3
O2 Cs2 Si1 103.31(7) . 3
O4 Cs2 Si1 95.89(10) 7_645 3
O1 Cs2 Si1 24.50(7) 3 3
O1 Cs2 Si1 64.53(7) 8_545 3
O5 U1 O5 180.0(2) 5_655 .
O5 U1 O1 90.02(16) 5_655 6
O5 U1 O1 89.98(16) . 6
O5 U1 O1 89.98(16) 5_655 2_655
O5 U1 O1 90.02(16) . 2_655
O1 U1 O1 180.0(4) 6 2_655
O5 U1 O1 90.02(16) 5_655 .
O5 U1 O1 89.98(16) . .
O1 U1 O1 87.7(2) 6 .
O1 U1 O1 92.3(2) 2_655 .
O5 U1 O1 89.98(16) 5_655 5_655
O5 U1 O1 90.02(16) . 5_655
O1 U1 O1 92.3(2) 6 5_655
O1 U1 O1 87.7(2) 2_655 5_655
O1 U1 O1 180.0(2) . 5_655
O5 U1 Cs2 55.25(17) 5_655 .
O5 U1 Cs2 124.75(17) . .
O1 U1 Cs2 53.69(11) 6 .
O1 U1 Cs2 126.31(11) 2_655 .
O1 U1 Cs2 53.69(11) . .
O1 U1 Cs2 126.31(11) 5_655 .
O5 U1 Cs2 124.75(17) 5_655 5_655
O5 U1 Cs2 55.25(17) . 5_655
O1 U1 Cs2 126.31(11) 6 5_655
O1 U1 Cs2 53.69(11) 2_655 5_655
O1 U1 Cs2 126.31(11) . 5_655
O1 U1 Cs2 53.69(11) 5_655 5_655
Cs2 U1 Cs2 180.0 . 5_655
O5 U1 U2 157.39(17) 5_655 .
O5 U1 U2 22.61(17) . .
O1 U1 U2 73.89(11) 6 .
O1 U1 U2 106.11(11) 2_655 .
O1 U1 U2 73.89(11) . .
O1 U1 U2 106.11(11) 5_655 .
Cs2 U1 U2 102.14(3) . .
Cs2 U1 U2 77.86(3) 5_655 .
O5 U1 U2 22.61(17) 5_655 5_655
O5 U1 U2 157.39(17) . 5_655
O1 U1 U2 106.11(11) 6 5_655
O1 U1 U2 73.89(11) 2_655 5_655
O1 U1 U2 106.11(11) . 5_655
O1 U1 U2 73.89(11) 5_655 5_655
Cs2 U1 U2 77.86(3) . 5_655
Cs2 U1 U2 102.14(3) 5_655 5_655
U2 U1 U2 180.000(7) . 5_655
O5 U1 Cs2 61.30(3) 5_655 7_655
O5 U1 Cs2 118.70(3) . 7_655
O1 U1 Cs2 44.94(12) 6 7_655
O1 U1 Cs2 135.06(12) 2_655 7_655
O1 U1 Cs2 119.32(12) . 7_655
O1 U1 Cs2 60.68(12) 5_655 7_655
Cs2 U1 Cs2 66.533(12) . 7_655
Cs2 U1 Cs2 113.467(12) 5_655 7_655
U2 U1 Cs2 112.646(13) . 7_655
U2 U1 Cs2 67.354(13) 5_655 7_655
O5 U1 Cs2 61.30(3) 5_655 7_645
O5 U1 Cs2 118.70(3) . 7_645
O1 U1 Cs2 119.32(12) 6 7_645
O1 U1 Cs2 60.68(12) 2_655 7_645
O1 U1 Cs2 44.94(12) . 7_645
O1 U1 Cs2 135.06(12) 5_655 7_645
Cs2 U1 Cs2 66.533(12) . 7_645
Cs2 U1 Cs2 113.467(12) 5_655 7_645
U2 U1 Cs2 112.646(13) . 7_645
U2 U1 Cs2 67.354(13) 5_655 7_645
Cs2 U1 Cs2 119.53(2) 7_655 7_645
O6 U2 O5 178.03(15) . .
O6 U2 O3 90.02(12) . 6
O5 U2 O3 88.55(15) . 6
O6 U2 O3 90.02(12) . .
O5 U2 O3 88.55(15) . .
O3 U2 O3 86.5(2) 6 .
O6 U2 O2 92.85(12) . 8_445
O5 U2 O2 88.58(16) . 8_445
O3 U2 O2 177.10(15) 6 8_445
O3 U2 O2 93.06(17) . 8_445
O6 U2 O2 92.85(12) . 3_455
O5 U2 O2 88.58(16) . 3_455
O3 U2 O2 93.06(17) 6 3_455
O3 U2 O2 177.10(15) . 3_455
O2 U2 O2 87.3(2) 8_445 3_455
O6 U2 U1 156.736(12) . .
O5 U2 U1 21.30(14) . .
O3 U2 U1 73.26(11) 6 .
O3 U2 U1 73.26(11) . .
O2 U2 U1 103.86(12) 8_445 .
O2 U2 U1 103.86(12) 3_455 .
O6 U2 Cs1 64.74(3) . .
O5 U2 Cs1 113.29(15) . .
O3 U2 Cs1 48.80(12) 6 .
O3 U2 Cs1 48.80(12) . .
O2 U2 Cs1 132.39(11) 8_445 .
O2 U2 Cs1 132.39(11) 3_455 .
U1 U2 Cs1 91.99(3) . .
O6 U2 Cs1 56.68(2) . 5_656
O5 U2 Cs1 125.29(15) . 5_656
O3 U2 Cs1 127.52(11) 6 5_656
O3 U2 Cs1 127.52(11) . 5_656
O2 U2 Cs1 54.82(11) 8_445 5_656
O2 U2 Cs1 54.82(11) 3_455 5_656
U1 U2 Cs1 146.582(19) . 5_656
Cs1 U2 Cs1 121.42(2) . 5_656
O6 U2 Cs2 124.687(12) . 3_445
O5 U2 Cs2 55.55(2) . 3_445
O3 U2 Cs2 128.68(11) 6 3_445
O3 U2 Cs2 60.33(12) . 3_445
O2 U2 Cs2 48.93(12) 8_445 3_445
O2 U2 Cs2 118.11(11) 3_455 3_445
U1 U2 Cs2 60.825(12) . 3_445
Cs1 U2 Cs2 108.891(19) . 3_445
Cs1 U2 Cs2 103.757(14) 5_656 3_445
O6 U2 Cs2 124.687(12) . 3_455
O5 U2 Cs2 55.55(2) . 3_455
O3 U2 Cs2 60.33(12) 6 3_455
O3 U2 Cs2 128.68(11) . 3_455
O2 U2 Cs2 118.11(11) 8_445 3_455
O2 U2 Cs2 48.93(12) 3_455 3_455
U1 U2 Cs2 60.825(12) . 3_455
Cs1 U2 Cs2 108.891(19) . 3_455
Cs1 U2 Cs2 103.757(14) 5_656 3_455
Cs2 U2 Cs2 109.65(2) 3_445 3_455
O6 U2 Cs1 64.807(14) . 3_455
O5 U2 Cs1 116.11(7) . 3_455
O3 U2 Cs1 76.40(12) 6 3_455
O3 U2 Cs1 149.07(12) . 3_455
O2 U2 Cs1 105.26(11) 8_445 3_455
O2 U2 Cs1 33.10(11) 3_455 3_455
U1 U2 Cs1 124.037(12) . 3_455
Cs1 U2 Cs1 101.806(17) . 3_455
Cs1 U2 Cs1 53.795(11) 5_656 3_455
Cs2 U2 Cs1 148.882(15) 3_445 3_455
Cs2 U2 Cs1 63.381(17) 3_455 3_455
O1 Si1 O2 113.1(2) . .
O1 Si1 O3 111.1(2) . .
O2 Si1 O3 110.3(2) . .
O1 Si1 O4 107.0(3) . .
O2 Si1 O4 108.2(3) . .
O3 Si1 O4 106.8(3) . .
O1 Si1 Cs1 168.19(16) . 7_646
O2 Si1 Cs1 78.51(17) . 7_646
O3 Si1 Cs1 60.77(16) . 7_646
O4 Si1 Cs1 69.6(3) . 7_646
O1 Si1 Cs1 115.30(18) . .
O2 Si1 Cs1 55.18(16) . .
O3 Si1 Cs1 58.19(16) . .
O4 Si1 Cs1 137.7(3) . .
Cs1 Si1 Cs1 68.91(3) 7_646 .
O1 Si1 Cs2 77.02(17) . 3_445
O2 Si1 Cs2 155.68(17) . 3_445
O3 Si1 Cs2 84.32(16) . 3_445
O4 Si1 Cs2 47.8(2) . 3_445
Cs1 Si1 Cs2 93.12(4) 7_646 3_445
Cs1 Si1 Cs2 142.49(4) . 3_445
O1 Si1 Cs2 49.53(16) . .
O2 Si1 Cs2 64.70(17) . .
O3 Si1 Cs2 119.87(17) . .
O4 Si1 Cs2 132.5(3) . .
Cs1 Si1 Cs2 141.09(5) 7_646 .
Cs1 Si1 Cs2 79.52(3) . .
Cs2 Si1 Cs2 125.68(5) 3_445 .
O1 Si1 Cs2 50.31(16) . 7_645
O2 Si1 Cs2 100.30(17) . 7_645
O3 Si1 Cs2 149.16(16) . 7_645
O4 Si1 Cs2 65.4(3) . 7_645
Cs1 Si1 Cs2 132.04(4) 7_646 7_645
Cs1 Si1 Cs2 147.55(4) . 7_645
Cs2 Si1 Cs2 68.36(4) 3_445 7_645
Cs2 Si1 Cs2 69.95(3) . 7_645
Si1 O1 U1 140.9(2) . .
Si1 O1 Cs2 107.4(2) . .
U1 O1 Cs2 92.06(14) . .
Si1 O1 Cs2 106.8(2) . 7_645
U1 O1 Cs2 106.17(15) . 7_645
Cs2 O1 Cs2 91.44(11) . 7_645
Si1 O1 Cs2 78.48(16) . 3_445
U1 O1 Cs2 89.13(13) . 3_445
Cs2 O1 Cs2 168.31(15) . 3_445
Cs2 O1 Cs2 77.07(10) 7_645 3_445
Si1 O2 U2 132.9(2) . 3_545
Si1 O2 Cs1 99.35(18) . .
U2 O2 Cs1 123.60(16) 3_545 .
Si1 O2 Cs2 91.00(18) . .
U2 O2 Cs2 102.73(14) 3_545 .
Cs1 O2 Cs2 94.58(11) . .
Si1 O2 Cs1 76.07(16) . 7_646
U2 O2 Cs1 95.50(14) 3_545 7_646
Cs1 O2 Cs1 75.30(9) . 7_646
Cs2 O2 Cs1 161.77(12) . 7_646
Si1 O3 U2 140.6(3) . .
Si1 O3 Cs1 95.98(18) . .
U2 O3 Cs1 99.60(15) . .
Si1 O3 Cs1 92.88(18) . 7_646
U2 O3 Cs1 124.93(17) . 7_646
Cs1 O3 Cs1 81.82(10) . 7_646
Si1 O4 Si1 143.3(4) . 6_545
Si1 O4 Cs2 108.2(2) . 3_445
Si1 O4 Cs2 108.2(2) 6_545 3_445
Si1 O4 Cs1 84.1(3) . 7_646
Si1 O4 Cs1 84.1(3) 6_545 7_646
Cs2 O4 Cs1 115.1(2) 3_445 7_646
Si1 O4 Cs2 90.4(3) . 7_645
Si1 O4 Cs2 90.4(3) 6_545 7_645
Cs2 O4 Cs2 82.67(18) 3_445 7_645
Cs1 O4 Cs2 162.2(2) 7_646 7_645
U1 O5 U2 136.1(3) . .
U1 O5 Cs2 92.9(2) . 5_655
U2 O5 Cs2 131.0(2) . 5_655
U2 O6 U2 180.0 5_656 .
U2 O6 Cs1 84.70(3) 5_656 5_656
U2 O6 Cs1 95.30(3) . 5_656
U2 O6 Cs1 95.30(3) 5_656 .
U2 O6 Cs1 84.70(3) . .
Cs1 O6 Cs1 180.0 5_656 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cs1 O2 3.100(4) .
Cs1 O2 3.100(4) 6
Cs1 O3 3.183(5) .
Cs1 O3 3.183(5) 6
Cs1 O3 3.208(4) 4_656
Cs1 O3 3.208(4) 7_646
Cs1 O4 3.461(8) 7_646
Cs1 O2 3.708(5) 4_656
Cs1 O2 3.708(5) 7_646
Cs2 O4 2.986(6) 3
Cs2 O1 3.145(4) .
Cs2 O1 3.145(4) 6
Cs2 O5 3.208(6) 5_655
Cs2 O1 3.211(4) 7_645
Cs2 O1 3.211(4) 4_655
Cs2 O2 3.567(5) 6
Cs2 O2 3.567(5) .
Cs2 O4 3.630(8) 7_645
Cs2 O1 3.807(4) 3
Cs2 O1 3.807(4) 8_545
Cs2 Si1 3.8280(18) 3
U1 O5 2.058(6) 5_655
U1 O5 2.058(6) .
U1 O1 2.196(4) 6
U1 O1 2.196(4) 2_655
U1 O1 2.196(4) .
U1 O1 2.196(4) 5_655
U1 U2 3.9305(8) .
U1 U2 3.9305(8) 5_655
U2 O6 2.1301(6) .
U2 O5 2.179(6) .
U2 O3 2.217(4) 6
U2 O3 2.217(4) .
U2 O2 2.246(4) 8_445
U2 O2 2.246(4) 3_455
Si1 O1 1.620(4) .
Si1 O2 1.624(4) .
Si1 O3 1.632(4) .
Si1 O4 1.637(2) .
O1 Cs2 3.211(4) 7_645
O1 Cs2 3.807(4) 3_445
O2 U2 2.246(4) 3_545
O2 Cs1 3.708(5) 7_646
O3 Cs1 3.208(4) 7_646
O4 Si1 1.637(2) 6_545
O4 Cs2 2.986(6) 3_445
O4 Cs1 3.461(8) 7_646
O4 Cs2 3.630(8) 7_645
O5 Cs2 3.208(6) 5_655
O6 U2 2.1301(6) 5_656
O6 Cs1 3.7891(10) 5_656
